Chennai, India. pp. 436 - 442.
Dispersion and Upgradation of Limestone from new Umrangshu, Assam, India
Bhaskar J. Sarmah, Pranjal Saikia', Prasanta J. Goutam, Pinaki Sengupta, Sekh Mahiuddin, Pradip C. Saikia and Prakash C. Borthakur2
Material Science Division, Regional Research Laboratory, Jorhat, Assam-785006, India.
Inorganic and Physical Chemistry Division, IICT, Hyderbad, India.
2 Corresponding author Email: firstname.lastname@example.org
North Cachor district of Assam, India is endowed with a vast deposit of limestone at New Umrangshu (25°31'51" to 25 '32'8" N latitude and 92°48'1" to 92 °48'7" E longitude). The deposit contains about 116 million tones of limestone extended over an area of 3.5 square km, which is used presently for manufacturing cement. The limestone contains over 91% CaCO3 (— 51-52% CaO) with —2.1-2.7% MgO, —1.5-2.2% Si02 and —0.8-0.9% A1203 mostly in the form of calcite with small to trace amounts of impurities like kaolinite, pyrite, illite. It was earlier reported that size classification leads only to marginal improvement of the limestone.
The coarser fraction contains the maximum amount of CaO and minimum amount of Si02, A1203 and Fe203,. whereas, the fine fraction contains the minimum amount of CaO and maximum amount of SiO2 and Fe,03. The impurities are evenly distributed in the limestone.
The present communication reports the results of further works carried on beneficiation of the limestone. Fine grinding leads to liberation of the clay minerals; the major impurities of the limestone which may be removed by adopting dispersion-cum-settling technique resulting a fraction containing —97% CaCO3 (54.3% CaO) with —0.5% SiO2 and —0.6% A1203.
Limestone is one of the most extensively exploited minerals. It finds use in manufacture of cement, building lime, paper, calcium carbide, bleaching powder, iron and steel, glass, ferro-alloys, fertilizers, rubber, toothpaste etc. The specifications of limestone for different purposes are different.
Almost all the states of NE region of India is endowed with vast deposits of limestone. R.R.L. Jorhat has. initiated a program to systematically characterize the prominent limestone deposits of the region to access their utility and possibility of value addition [1,2]. Directorate of Geology and Mining, Govt.
of Assam proved a limestone deposit containing about 116 million tones of limestone in a 3.5 square km area in New Umrangshu, North Cachar Hills, Assam (25°31'51" to 25°32'8" N latitude and 92°48'1" to 92°48'7" E longitude).
In an earlier communication  we reported the physicochemical characteristics of the limestone and possibility of upgrading the same by dry beneficiation technique. The limestone contains over 51%
CaO and mineralogically it is calcite contaminated with small to trace amount of clay minerals, of which kaolinite is the major phase. Size classification reveals that the coarser fraction contains the maximum amount of CaO (51.79%) and minimum amount of Si02 (1.53%), and A1203 (0.79%) whereas, the fine fraction contains the minimum amount of CaO (50.92%) and maximum amount of Si02 (2.25%). The present communication reports the results of further works carried on upgrading the limestone by fine grinding followed by separation using dispersion cum settling technique.
MATERIALS AND METHODS
About 10 tones of limestone were procured from New Umrangshu deposit through Assam Mineral Development Corporation, Govt. of Assam, Guwahati. It was then subjected to size reduction in a jaw crusher followed by separation in to three fractions: —25mm+18.75mm, —18.75+12.5mm and — 12.5mm, which are marked as ULA, ULB and ULC respectively. A representative sample ULR, prepared by mixing the different sized fractions in the same proportions as obtained during crushing was further pulverized to —150gm size in a planetary ball mill. A suspension (2 liter) of the pulverized representative sample in water 1% (w/v) was subjected to stirring (14 000 rpm) in a Hamilton beach mixture (NL Baroid, USA, Model 936-31S-1) in presence of dispersing agents (-1.0 g of (NaPO3)6 and —0.1 g Na2CO3). The suspension (pH — 8.5) was then transferred to a cylindrical column and allowed to settle the +70 gm fraction by maintaining the appropriate sedimentation time worked out as per Stoke's law. The sediment was collected and dried at 100±10 °C. The dispersed phase was further separated into three different size fractions (viz. — —70 pm + 20 tun, — —20 gm + 2 gm and — — 2 gm) by adopting dispersion cum settling technique and using Stoke's law and the separated fractions were washed and dried at 100±10 °C. The procedure adopted for processing the limestone is schematically shown in Fig. 1.
Umrangsu Limestone I
Size classification after crushing in a jaw crusher
ULA (-25mm+18.75mm) ULB (-18.75mm+12mm) ULC (—I2mm)
Ground to — 150 pm size.
Dispersed in water, stirred and processed using dispersing agent.
Sediment phase (-470 pm)
Coarse Part, dried at 100 °C and collected
Fractionation into various size fractions using dispersion cum settling technique and Stoke's law.
Fraction 1 (— -70+ 20 pm)
Fraction 2 20 pm+ 2 pm)
Fraction 3 (— - 2 pm)
Fig. 1: Scheme for Recovering Various Fractions of Limestone Sample
The chemical analyses of the samples were done by standard methods of analysis . The CaO, MgO and Fe2O3 contents were determined volumetrically using EDTA for the former two and potassium dichromate as oxidant for the later. The amount of SiO2 and A1203 were estimated gravimetrically.
Mineralogical characterization of the limestone sample and it's size fractions were performed using XRD analysis of random powder samples (Philips X-ray Diffractometer, Type PW1710, UK and Brucker D8 advance XPS, Germany) using Cu Kr, X-radiation; Thermal analysis (TA instrument, model STD 2960, USA) under air flow rate of 100 ml/min, heating rate of 10 °C/min up to 1000 °C
and using calcined a-A1203 as the reference material in a platinum crucible; FTIR (Perkin Elmer System 2000 spectrophotometer, USA) using KBr pellet method; SEM (model LEO 5430) coupled with EDXA (LINK ISIS, OXFORD INSTRUMENTS, UK) and particle size analysis (Laser Particle Size Analyser, Model CILAS 1180, France).
RESULTS AND DISCUSSIONS
The yield and chemical analyses of different size fractions obtained by processing the limestone sample are shown in Tables 1 and 2 respectively.
Table 1: Percentage Yield of Various Fractions Obtained on Processing of the Limestone Fractions. Yield (% w/w)
Coarse Part 57.23 Fraction I 11.83 Fraction 2 25.02
Fraction 3 5.88
Table 2: Chemical Compositions of Feed Limestone ULR and its Fractions Size
Chemical Composition (% w/w)
CaO MgO Si02 A1203 Fe203 LOI
ULR 51.75 2.57 1.70 0.83 0.81 41.50
Coarse Part 52.60 1.97 0.51 1.02 0.95 42.03
Fraction 1. 54.28 1.10 0.53 0.62 0.71 42.53
Fraction 2. 53.35 0.96 0.55 0.65 0.78 42.16
It is observed that the Coarse part contains about 57.23% of the limestone and its CaO and A1203 content is higher and Si02 and MgO contents are lower than the parent sample ULR. Its Si02 content (0.51%) is comparable to that of Fraction 1 and Fraction 2 and much lower than that in the parent sample (1.70%). Similarly the Fractions 1 and 2 contain higher amount of Ca0 (54.28-53.35%) and lower amount of A1203 than the parent sample. The Fe203 contents of all the fractions are comparable with that of the parent sample. Pulverization of the limestone followed by wet separation using dispersion cum settling technique leads to liberation and separation of the clay minerals present in it leading to a limestone fraction enriched with CaO.
The XRD pattern of the parent sample ULR is given in Fig. 2. The sample contains calcite (d=3.84, 3.02, 2.81, 2.47, 1.91, 1.59, A) as the major phase. The XRD pattern of the Coarse part (Fig. 3.) indicates presence of Boehmite (d=6.2, 3.17, 2.35 A), Goethite (d= 4.16, 2.68, 2.44 A), Siderite (d=2.82, 1.74, 1.73 A) and Pyrite (d=2.72, 2.42, 1.61 A) in addition to Calcite (d=3.84, 3.02, 2.84, 2.48 A).
Isamr1. tarartit .t,..
LOSS CC uuuuu 1 •
Fig. 2: XRD Pattern of ULR Sample
Fig. 3: XRD Pattern of Coarse Part
The XRD patterns of Fractions 1 and 2 (Patterns not shown) also show paeks at d =3.84, 3.02, 2.84, 2.48, 1.91, 1.86, 1.59 A due to calcite with small peaks for pyrite 1.91, 1.62 and 1.44 A), Kaolinite (c1=7.15, 3.58, 1.49 A) and Illite (d=4.46, 3.34,2.55 A).
The XRD pattern of Fraction 3 (Fig. 4.) reveals the presence of Kaolinite (d=7.15, 3.58, 1.49 A) as the major phase, with small peaks due to Illite, Calcite and Pyrite. Peaks due to Boefunite, Goethite and Siderite are not observed in the patterns of Fractions 1, 2 and 3 .
288 Z59 288 152 188 58
20 48 S.
Fig. 4: XRD Pattern of Fraction 3
The particle size of the parent sample ULR ranges from 0.04 to 260 gm with (Table 3) the mean diameter of 57.46 gm. The Coarse part contains particles of even less than +70 gm size (32 % material). It is possible that Pyrite, Goethite, Boehmite etc. heavy minerals (as reveled by XRD) exist in the fraction which might be of finer size. The fraction 1 and Fraction 2 also contain particles finer than the targeted +20 gm and +2 gm size respectively. The latter may be due to clay minerals. On the other hand, Fraction 3 contains 66.43% particles in the size range -70 Inn +2 gm. This indicates that many of the fine and medium sized limestone particles get dispersed under the condition and composition employed for dispersion. Optimization of dispersant dosage and composition may lead to selective separation of the particles.
Table 3: Particle Size Distributions in Different Size Fractions
Particle size range
Diameter m) at cumulative %
90 70 50 30 10
Coarse Part 0.07-260 96.33 162.54 122.2 96.43 66.32 29.70 Fraction 1 0.07-71.00 17.09 32.02 22.10 16.24 10.50 1.42 Fraction 2 0.07-12.00 3.70 7.86 5.10 3.14 1.70 0.38 Fraction 3 0.04-71.00 13.98 36.01 20.10 9.17 1.70 0.66
ISO 265 abo Soo ode 700 *do 060 tom"
Fig. 5: Thermal Curves of Coarse Part, (A) TG (B) DTA, (C) DTG
0 200 400 600 800 1000
Fig. 6: Thermal Curve of Fraction 3 (A) TG, (B) DTA, (C) DTG 60
•0.02 0.10 0.08 0.06 0.04 0.02 - 0.00 0.02
Dispersion and Upgradation ofLimestone from new Umrangshu, Assam, India
Thermal analysis pattern of the Coarse part is shown in Fig. 5. The DTA curve of the coarse fraction exhibits sharp endotherm at 600-800 °C temperature regions with peak at around 770 °C, accompanied by weight loss in TG and DTG curve is attributed to decarbonation of the limestone. The thermal curves of Fraction 3 (Fig. 6.) show weak endothermic trend accompanied by weight loss at around 100 °C, attributed to dehydration of clay minerals. The endothermic peak at around 500 °C accompanied by weight loss in TG and DTG curves indicate dehydroxylation of kaolinite. Exothermic trend noted above 850 °C is also characteristics of some clay minerals. The pattern also exhibits a weak endotherm at .650 °C, which may be due to calcite. The drop in decarbonation temperature from 750 to 650 °C may be due to the fineness of the particles and presence of other materials as the major phase [5,6].
1000 2000 3000 4000
wave number(cm -1 )
Fig. 7: FTIR Spectra of (A) ULR and (B) Coarse Part
The FTIR spectra of parent sample ULR and Coarse part are shown in Fig. 7. In the spectra, IR bands at —713, 876, 1427 and 2514 cnil are diagnostic bands for calcite. The weak peaks at —470 and 537
Proceedings of the International Seminar on Mineral Processing Technology cm'
cm are assigned for •Si-0 asymmetric bending vibrations of quartz, feldspar and other alumino/aluminiumsilicate group of minerals. Small peak at —913 cm' is due to Al...0-H - vibrations.
Bands at 1008 and 1032 cm' are indicative of vsi.0 vibration. The peaks at —1084 and 1112 cm' are due to v. vibrations of Si-O-Si. Presence of water in the sample is revealed by peaks at —3447 and 1799
cm'. The small peaks at the region —2598 — 2983
cmmay be for organic matters present in the sample.
The FTIR spectra of Fraction 3 (Fig. 8) exhibits sharp peaks at —470, 537, 753, 913, 1032, 1108, 3694 and 3620 cm', characteristics of the clay mineral kaolinite. Band in the region —1430 cm' indicates presence of carbonate bearing minerals .
1000 2000 3000 4000
wavenum ber (cm") Fig. 8: FTIR Spectra of Fraction 3
The SEM-EDXA pattern of Fraction 3 (Fig. 9) shows combination of plate like, layered and irregular shaped flaked particles characteristics of clay minerals . The EDXA data also suggest presence of clay minerals and aluminosilicate in addition to calcite.
Fig. 9: SEM-EDXA of Fraction 3 CONCLUSIONS
The clay minerals present as the major impurity in Umrangshu limestone are liberated by fine grinding and are separated by adopting dispersion cum settling technique. A limestone fraction (-12%) with —97% CaCO3 may be obtained from the parent sample containing —91% CaCO3. It may be possible to improve the yield and quality of the limestone fractions by optimizing the grinding parameters, nature and dose of the dispersing agent etc.
The authors are grateful to Department of Mines, Ministry of Coal and Mines, Govt. of India, New Delhi for financial grant and also to Directorate, Geology and Mining, Govt. of Assam and Assam Mineral Development Corporation for their help in procurement of the limestone sample. The authors are also grateful to Dr. P. G. Rao, Director, RRL, Jorhat for his interest and support.
Saikia P., Sarmah B. J., Mahiuddin S., Sengupta P., Saikia P. C., Bordoloi D., and Borthakur P.
C., 2005, "Limestone from New Umrangshu, Assam, India: Characterisation and utilisation prospects," Procd. Int. Seminar on Mineral Processing Technology (MPT- 2005), pp 187-193.
Sarmah B. J, Saikia P., Mahiuddin S., Sengupta P., Saikia P. C., Bordoloi D., and Borthakur P.C., 2005 "Physicochemical characteristics of Limestone from Lumshnong, Jayantia Hills, Meghalaya," Procd. Int. Conference on Emerging Trends in Mineral Processing and Extractive Metallurgy (ICME-2005), pp 111-116.
Vogel A. I., 1961, A Text Book of Quantitative Inorganic Analysis including Elementary Instrumental Analysis, ELBS and Longman, London.
Powder Diffraction File, PC-PDF File No. 5-0586, International Centre for Diffraction Data.
Mackenzie, R. C., 1970, Differential Thermal Analysis, Academic press, London.
Bensted, J. and Barnes, P., 2002, Structure and Performance of Cements, 2nd ed., Spon Press, NewYork.
Ramasamy, V., Anandalakshmi, K and Pounysamy V., 2003. Indian J. Phys 77A (4), pp.
Russell J. D., and Fraser A. R., 1994, Infrared methods. In: Wilson, M. J. (Ed), Clay Mineralogy: Spectroscopic and chemical determinative methods, Chapman and Hall, London, pp 1-67.
Grim, R. E., Clay Mineralogy, Vd ed., 1968, McGraw Hill, London p.106 and 212.